thermal expansion of l-ascorbic acid .thermal expansion of l-ascorbic acid ... iut orsay,...
Post on 02-Jul-2018
Embed Size (px)
THERMAL EXPANSION OF L-ASCORBIC ACID
B. Nicolaa,*, M. Barrio
b, J.-Ll. Tamarit
b, R. Colin
c, I.B. Rietveld
a Caracterisation des Matriaux Molculaires Activit Thrapeutique (CAMMAT), Facult de
Pharmacie, Universit Paris Descartes, 75006 Paris, France
b Grup de Caracteritzacio de Materials (GCM), Departament de Fisica i Enginyeria Nuclear,
Universitat Politecnica de Catalunya, ETSEIB, 08028 Barcelona, Spain
cLETIAM, EA7357, IUT Orsay, universit Paris Sud, rue Noetzlin, 91405 Orsay Cedex
* Corresponding author: firstname.lastname@example.org
Abstract The specific volume of vitamin C has been investigated by X-ray powder diffraction as a
function of temperature from 110 K up to complete degradation around 440K. Its thermal
expansion is relatively small in comparison with other organic compounds with an expansivity v
of 1.2(3) 10-4
. The structure consists of strongly bound molecules in the ac plane through a
dense network of hydrogen bonds. The thermal expansion is anisotropic. Along the b axis, the
expansion has most leeway and is about 10 times larger than in the other directions.
1 Introduction As mentioned in the paper on the thermodynamic origin of phase diagrams by Colin and
Rietveld in this special issue , temperature volume (T-v) phase diagrams are the projections
of the intersections of the tangential lines connecting the Helmholtz free energy surfaces for the
different phases of a system. Thus, the thermal expansion of a solid represents its T-v equilibrium
with its vapor phase, which is part of the larger picture of the phase behavior of a chemical
substance, which can be depicted as derivations of the Gibbs, Helmholtz, and internal energy and
the enthalpy. Although it is not common to present phase behavior in the form of T-v phase
diagrams, as pressure-temperature phase diagrams are more commonly used, certain systems do
benefit from the T-v representation, in particular if their vapor pressure is significant, such as for
the organic compound camphor  and the metalloid arsenic .
L-ascorbic acid or vitamin C is known for its antiscorbutic and antioxidant properties. It is a
labile water-soluble compound that degrades on heating and even in air at room temperature. In
addition, it is known to degrade on storage in solution at room temperature. The influence of
temperature on the chemical stability of L-ascorbic acid has mainly been studied in solution and
thermal decomposition has rarely been studied in the solid state; only calorimetric and
gravimetric data are available in the literature [4,5]. In addition, although the crystal structure of
vitamin C is known for years , both from single-crystal X-ray and neutron diffraction
measurements at and below room temperature [6-13], the influence of heating on crystalline L-
ascorbic acid has never been studied by X-ray diffraction.
A search in the Cambridge Structural Database (CSD) for crystal structures of L-ascorbic
acid resulted in a number of structure files that all contained the same space group and unit cell.
The references of the most useful CSD files have been compiled in Table 1 together with a few
other publications on the structure [6-11]. L-ascorbic acid crystallizes in the monoclinic system
with the non-centrosymmetric space group P21, with 4 molecules per unit-cell (Z = 4). In
addition, several possible structures of L-ascorbic acid have been found by a number of different
simulation approaches . Some of those have an energy relatively close to the known structure
, so it would be interesting to investigate by temperature dependent X-ray diffraction whether
transient phases could be observed.
A possible degradation product of L-ascorbic acid through dimerization is dehydro-L-
ascorbic acid, which crystallizes in the monoclinic system as well, with space group C2 and with
two dimers in the unit cell (Z = 2). A preliminary report on its crystal structure was published by
Hvoslef , who later published a complete description of the structure . Literature data has
been compiled in Table 1.
The thermal behavior of L-ascorbic acid, presented in this paper, will be used to
investigate the presence of any transient structures on heating. Furthermore, the intermolecular
interactions in the crystal of L-ascorbic acid will be investigated with the help of the thermal
expansion tensor in combination with its structural characteristics such as hydrogen bonds.
Figure 1. L-ascorbic acid or vitamin C, C6H8O6, (R)-3,4-dihydroxy-5-((S)-1,2
dihydroxyethyl)furan-2(5H)-one, M = 176.12 g mol-1
Table 1. Crystal data in the literature of L-ascorbic acid and dehydro-L-ascorbic acid
a CSD: Cambridge Structural Database
b RT is room temperature (283 303 K)
T/K a / b / c / / V /3 Ref / CSD
RTb 17.20 6.37 6.40 10205 685.67 
RTb 17.299(8) 6.353(3) 6.411(3) 102.18(13) 688.712 [7,8] / LASCAC01, 10
120 6.390(1) 6.262(1) 17.127(4) 99.36(2) 676.198  / LASCAC12
100 6.395(2) 6.240(2) 17.095(3) 99.341(9) 673.129  / LASCAC13
100 6.396(6) 6.242(2) 17.099(10) 99.33(4) 673.627  / LASCAC14
dehydro-L-ascorbic acid (C12H12O12, M = 348.22 g mol-1
RTb 15.69 5.55 9.47 130.2 629.86 
RTb 15.728(9) 5.530(2) 9.453(5) 130.56(4) 624.64 
2.1 Vitamin C L-ascorbic acid of a purity 99% was purchased from Sigma-Aldrich. It is a white powder,
which was used as such for the experiments after initial X-ray measurements demonstrated that
its diffraction pattern was identical to the one calculated from the CIF file in the Cambridge
Structural Database (CSD ref LASCAC10) with no extra peaks .
2.2 High resolution X-ray powder diffraction A Debye-Scherrer geometry was used in combination with an INEL X-ray powder
diffractometer equipped with a cylindrical position-sensitive detector (CPS120) containing 4096
channels (0.029 2 angular step) and monochromatic Cu K1 ( = 1.54061 ) radiation.
For the measurements as a function of temperature, a liquid nitrogen 700 series Cryostream
Cooler from Oxford Cryosystems (UK) was used. Slightly ground specimens were introduced in
a Lindemann capillary (0.5 mm diameter) rotating perpendicularly to the X-ray beam during the
experiments to improve the average over the crystallite orientations. The temperature-dependent
measurements were carried out from 110 K up to 440 K, while the sample temperature was
allowed to equilibrate for 10 min after changing the temperature to a new value. The heating rate
in between data collection was 1.33 K min-1
. The X-ray powder diffraction data were analyzed
with the software FULLPROF using pattern matching .
2.3 Isobaric thermal expansion tensor The anisotropy of the intermolecular interactions was investigated with the isobaric thermal
expansion tensor, which is a measure of how the interactions change with temperature . The
tensor was calculated from the temperature-dependent lattice parameters with the program
DEFORM . Details of the procedure for the calculation of the tensor have been published
Decomposition of the tensor matrix yields the magnitude (eigenvalue) and orientation
(eigenvector) of the thermal expansion along the 3 principal axes, e1, e2, and e3. The tensor
indicates the directions of the least and most deformation as a function of temperature and these
directions are commonly referred to as hard and soft directions, respectively, because they are
related to the intermolecular interactions. The anisotropy of the thermal expansion of the
intermolecular interactions can be condensed in the aspherism coefficient A [18,22,23].
Graphical representations of the tensor at given temperatures have been drawn using Wintensor
3 Results The diffraction patterns obtained as a function of temperature from 110 up to 440 K can be
seen in Figure 2. Indexing of the patterns has led to the temperature dependence of the lattice
parameters (See Table S1 in the Supplementary Information), which are linear except for
parameter c, which has been fitted with a quadratic function.
Figure 2. The diffraction patterns of vitamin C from 110 K up to 440 K. At 440 K, the sample
partly degrades into a non-crystalline material, as indicated by the upward curvature of the
a / = 17.243(2) + 1.69(8) 10-4 T/K (r2 = 0.983) (1)
b / = 6.175(4) + 6.09(12) 10-4 T/K (r2 = 0.997) (2)
c / = 6.3929(12) + 2.6(9) 10-5 T/K + 9.4(1.6) 10-8 T2/K2 (r2 = 0.997) (3)
, the only non-90 angle in the monoclinic cell, remains virtually constant with an average value
of 102.08(4). The extremes are 102.125(1) at 110 K and 102.015(4) at 440 K. The volume of the
unit-cell, V, is very similar to the literature data and its change as a function of temperature was
found to be linear as well:
V/ 3 = 664.5(6) + 0.0821(20) T/K (r2 = 0.995) (4)
With eq. 4, the expansivity of L-ascorbic acid, V, can be calculated, defined as V = V0 (1 + V T).
V0 = 664.5(6) 3, which has been obtained from eq. 4 and this leads to a value for V of 1.2(3)
The unit-cell data ha